#------------------------------------------------------------------------------
#$Date: 2025-07-01 14:18:43 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1222 $
#$URL: svn://crystallography.net/testcod/cif/4/00/00/4000027.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4000027
loop_
_publ_author_name
'Martín-Sedeño, M. C.'
'Losilla, E. R.'
'León-Reina, L.'
'Bruque, S.'
'Marrero-López, D.'
'Núñez, P.'
'Aranda, M. A. G.'
_publ_section_title
;
 Enhancement of Oxide Ion Conductivity in Cuspidine-Type Materials
;
_journal_issue                   24
_journal_name_full               'Chemistry of Materials'
_journal_page_first              4960
_journal_page_last               4968
_journal_paper_doi               10.1021/cm0487472
_journal_volume                  16
_journal_year                    2004
_chemical_formula_sum            'Ga0.35 Ge0.15 La O2.33'
_chemical_formula_weight         211.40
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_audit_creation_date             2004-07-01T15:57
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2004-07-01T15:57  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 110.175(5)
_cell_angle_gamma                90.0
_cell_formula_units_Z            16
_cell_length_a                   8.06422(17)
_cell_length_b                   11.15783(27)
_cell_length_c                   11.6910(5)
_cell_volume                     987.40(6)
_computing_structure_refinement  GSAS
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     1.886
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  1.00000
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 No correction is applied.
;
_pd_block_id
2004-07-01T15:57|La4(Ga14Ge06O73)O2_773K|M.A.G.Aranda|HRPT_773K
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        4.0
_pd_meas_2theta_range_max        0.0
_pd_meas_2theta_range_min        4.0
_pd_phase_name                   'from LaGaGe_rt.gsa '
_pd_proc_2theta_range_inc        4.0
_pd_proc_2theta_range_max        -0.01
_pd_proc_2theta_range_min        3.99
_pd_proc_info_datetime           2004-07-01T15:57:13
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 7 with 36 terms.
 Linear interpolation
      1:    4646.76     2:    4347.78     3:    4549.92     4:    4647.33    
      5:    4838.44     6:    4877.88     7:    5802.32     8:    5192.32    
      9:    5313.88    10:    5852.02    11:    6548.72    12:    7027.15    
     13:    6435.66    14:    6471.32    15:    6504.54    16:    5896.87    
     17:    6322.28    18:    6735.65    19:    7306.91    20:    7511.67    
     21:    7425.49    22:    7676.87    23:    7394.50    24:    7790.49    
     25:    7505.84    26:    7479.74    27:    8845.57    28:    8484.96    
     29:    7238.79    30:    8102.69    31:    7831.16    32:    7702.90    
     33:    7947.63    34:    7929.90    35:    7328.47    36:    8035.21    
;
_pd_proc_ls_peak_cutoff          0.00500
_pd_proc_ls_profile_function
;
 CW Profile function number 2 with  18 terms
 Profile coefficients for Simpson's rule integration of pseudovoigt function
 C.J. Howard (1982). J. Appl. Cryst.,15,615-620.
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 #1(GU)   =  218.647 #2(GV)   = -644.925 #3(GW)   =  609.039
 #4(LX)   =    0.000 #5(LY)   =   13.377 #6(trns) =    0.000
 #7(asym) =   3.4686 #8(shft) =   0.0000 #9(GP)   =    0.000
 #10(stec)=     0.00 #11(ptec)=     0.00 #12(sfec)=     0.00
 #13(L11) =    0.000 #14(L22) =    0.000 #15(L33) =    0.000
 #16(L12) =    0.000 #17(L13) =    0.000 #18(L23) =    0.000
 Peak tails are ignored  where the intensity is below 0.0050 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0178
_pd_proc_ls_prof_wR_expected     0.0106
_pd_proc_ls_prof_wR_factor       0.0228
_pd_spec_mounting                ' ?'
_refine_ls_goodness_of_fit_all   2.25
_refine_ls_matrix_type           full
_refine_ls_number_parameters     110
_refine_ls_number_restraints     0
_refine_ls_R_Fsqd_factor         0.06214
_refine_ls_shift/su_max          0.04
_refine_ls_shift/su_mean         0.00
_reflns_d_resolution_high        0.966
_reflns_d_resolution_low         7.824
_reflns_limit_h_max              8
_reflns_limit_h_min              0
_reflns_limit_k_max              11
_reflns_limit_k_min              0
_reflns_limit_l_max              11
_reflns_limit_l_min              -12
_reflns_number_observed          984
_cod_data_source_file            cm0487472si20040730_045737.cif
_cod_data_source_block           La4(Ga14Ge06O73)O2_773K_publ
_cod_original_cell_volume        987.40308
_cod_database_code               4000027
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -x,+y+1/2,-z+1/2
-1 -x,-y,-z
-2 +x,-y+1/2,+z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
GA Ga1 0.1585(17) 0.1896(14) 0.1240(13) 0.7 Uiso 0.016(4) 4
GA Ga2 0.6781(22) 0.1932(13) 0.1243(13) 0.7 Uiso 0.020(4) 4
LA La1 0.5272(24) 0.0910(15) 0.7964(13) 1.0 Uiso 0.020(4) 4
LA La2 0.0325(19) 0.0871(13) 0.8026(11) 1.0 Uiso 0.0107(33) 4
LA La3 0.3463(19) 0.1280(12) 0.4234(12) 1.0 Uiso 0.0061(30) 4
LA La4 0.8411(22) 0.1246(12) 0.4262(12) 1.0 Uiso 0.0069(33) 4
O O1 0.7951(25) 0.2231(18) 0.7598(19) 1.0 Uiso 0.030(6) 4
O O2 0.2371(23) 0.2099(15) 0.7586(15) 1.0 Uiso 0.016(4) 4
O O3 0.2154(27) 0.0409(12) 0.1847(11) 1.0 Uiso 0.009(4) 4
O O4 0.0966(26) 0.2345(22) 0.9659(16) 1.0 Uiso 0.021(5) 4
O O5 0.440(4) 0.2224(20) 0.1232(21) 0.76(4) Uiso 0.0343(30) 4
O O6 0.613(4) 0.2301(25) 0.9770(20) 1.0 Uiso 0.040(6) 4
O O7 0.7120(35) 0.0368(16) 0.1574(15) 1.0 Uiso 0.044(6) 4
O O8 0.0868(29) 0.0010(17) 0.4006(19) 1.0 Uiso 0.021(5) 4
O O9 0.5721(23) 0.0052(13) 0.3948(16) 1.0 Uiso -0.0023(35) 4
GE Ge1 0.1585(17) 0.1896(14) 0.1240(13) 0.3 Uiso 0.016(4) 4
GE Ge2 0.6781(22) 0.1932(13) 0.1243(13) 0.3 Uiso 0.020(4) 4
O O10 0.072(7) 0.7474(28) 0.3859(32) 0.54(4) Uiso 0.0343(30) 4
loop_
_atom_type_symbol
_atom_type_number_in_cell
_atom_type_scat_length_neutron
_atom_type_scat_source
GA 5.6 0.7288 International_Tables_Vol_C
LA 16.0 0.8240 International_Tables_Vol_C
O 37.2 0.5803 International_Tables_Vol_C
GE 2.4 0.8185 International_Tables_Vol_C
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Ga1 O3 104.8(11) -2_565 . 1_555 N
O2 Ga1 O4 126.3(13) -2_565 . 1_554 N
O2 Ga1 O5 81.9(9) -2_565 . 1_555 N
O2 Ga1 O10 83.7(13) -2_565 . 2_545 N
O3 Ga1 O4 126.9(13) 1_555 . 1_554 N
O3 Ga1 O5 91.7(10) 1_555 . 1_555 N
O3 Ga1 O10 116.0(14) 1_555 . 2_545 N
O4 Ga1 O5 83.0(10) 1_554 . 1_555 N
O4 Ga1 O10 85.8(13) 1_554 . 2_545 N
O5 Ga1 O10 151.2(13) 1_555 . 2_545 N
O1 Ga2 O5 97.8(12) -2_565 . 1_555 N
O1 Ga2 O6 131.5(14) -2_565 . 1_554 N
O1 Ga2 O7 108.8(11) -2_565 . 1_555 N
O1 Ga2 O10 71.6(12) -2_565 . 2_645 N
O5 Ga2 O6 89.5(13) 1_555 . 1_554 N
O5 Ga2 O7 104.0(13) 1_555 . 1_555 N
O5 Ga2 O10 153.7(11) 1_555 . 2_645 N
O6 Ga2 O7 115.8(14) 1_554 . 1_555 N
O6 Ga2 O10 80.9(16) 1_554 . 2_645 N
O7 Ga2 O10 102.2(14) 1_555 . 2_645 N
O1 La1 O2 114.1(7) 1_555 . 1_555 N
O1 La1 O3 69.9(7) 1_555 . -1_656 N
O1 La1 O5 60.6(9) 1_555 . -2_566 N
O1 La1 O6 78.4(9) 1_555 . 1_555 N
O1 La1 O7 176.8(9) 1_555 . -1_656 N
O1 La1 O9 97.1(8) 1_555 . -1_656 N
O2 La1 O3 173.3(9) 1_555 . -1_656 N
O2 La1 O5 60.8(8) 1_555 . -2_566 N
O2 La1 O6 78.3(8) 1_555 . 1_555 N
O2 La1 O7 68.0(8) 1_555 . -1_656 N
O2 La1 O9 94.6(7) 1_555 . -1_656 N
O3 La1 O5 119.5(9) -1_656 . -2_566 N
O3 La1 O6 108.1(10) -1_656 . 1_555 N
O3 La1 O7 108.3(7) -1_656 . -1_656 N
O3 La1 O9 79.3(7) -1_656 . -1_656 N
O5 La1 O6 94.3(7) -2_566 . 1_555 N
O5 La1 O7 122.4(10) -2_566 . -1_656 N
O5 La1 O9 74.7(7) -2_566 . -1_656 N
O6 La1 O7 99.9(10) 1_555 . -1_656 N
O6 La1 O9 168.9(10) 1_555 . -1_656 N
O7 La1 O9 85.1(8) -1_656 . -1_656 N
O1 La2 O2 99.2(7) 1_455 . 1_555 N
O1 La2 O3 76.9(7) 1_455 . -1_556 N
O1 La2 O4 70.7(7) 1_455 . 1_555 N
O1 La2 O7 175.0(10) 1_455 . -1_656 N
O1 La2 O8 91.9(9) 1_455 . -1_556 N
O1 La2 O10 53.1(11) 1_455 . -1_566 N
O2 La2 O3 171.0(7) 1_555 . -1_556 N
O2 La2 O4 78.5(8) 1_555 . 1_555 N
O2 La2 O7 75.8(8) 1_555 . -1_656 N
O2 La2 O8 95.3(8) 1_555 . -1_556 N
O2 La2 O10 58.6(12) 1_555 . -1_566 N
O3 La2 O4 107.3(8) -1_556 . 1_555 N
O3 La2 O7 108.1(7) -1_556 . -1_656 N
O3 La2 O8 76.9(7) -1_556 . -1_556 N
O3 La2 O10 113.3(12) -1_556 . -1_566 N
O4 La2 O7 107.5(8) 1_555 . -1_656 N
O4 La2 O8 160.1(9) 1_555 . -1_556 N
O4 La2 O10 95.6(9) 1_555 . -1_566 N
O7 La2 O8 89.0(8) -1_656 . -1_556 N
O7 La2 O10 123.2(13) -1_656 . -1_566 N
O8 La2 O10 65.5(8) -1_556 . -1_566 N
O2 La3 O3 65.3(6) -2_565 . 1_555 N
O2 La3 O4 69.8(7) -2_565 . -2_565 N
O2 La3 O5 97.6(7) -2_565 . -2_566 N
O2 La3 O6 77.9(8) -2_565 . -2_565 N
O2 La3 O8 105.4(9) -2_565 . 1_555 N
O2 La3 O9 112.3(8) -2_565 . 1_555 N
O2 La3 O9 169.4(8) -2_565 . -1_656 N
O3 La3 O4 109.3(7) 1_555 . -2_565 N
O3 La3 O5 162.8(8) 1_555 . -2_566 N
O3 La3 O6 117.0(8) 1_555 . -2_565 N
O3 La3 O8 71.2(7) 1_555 . 1_555 N
O3 La3 O9 72.8(7) 1_555 . 1_555 N
O3 La3 O9 122.9(7) 1_555 . -1_656 N
O4 La3 O5 60.4(8) -2_565 . -2_566 N
O4 La3 O6 102.6(7) -2_565 . -2_565 N
O4 La3 O8 71.8(8) -2_565 . 1_555 N
O4 La3 O9 177.6(9) -2_565 . 1_555 N
O4 La3 O9 100.1(7) -2_565 . -1_656 N
O5 La3 O6 57.2(8) -2_566 . -2_565 N
O5 La3 O8 114.5(9) -2_566 . 1_555 N
O5 La3 O9 117.8(10) -2_566 . 1_555 N
O5 La3 O9 73.9(7) -2_566 . -1_656 N
O6 La3 O8 171.6(10) -2_565 . 1_555 N
O6 La3 O9 77.0(8) -2_565 . 1_555 N
O6 La3 O9 102.0(8) -2_565 . -1_656 N
O8 La3 O9 108.3(7) 1_555 . 1_555 N
O8 La3 O9 73.4(8) 1_555 . -1_656 N
O9 La3 O9 77.7(7) 1_555 . -1_656 N
O1 La4 O4 67.1(7) -2_565 . -2_665 N
O1 La4 O6 80.4(8) -2_565 . -2_565 N
O1 La4 O8 101.0(8) -2_565 . 1_655 N
O1 La4 O8 172.3(10) -2_565 . -1_656 N
O1 La4 O9 111.3(8) -2_565 . 1_555 N
O1 La4 O10 102.4(10) -2_565 . -1_666 N
O4 La4 O6 99.4(7) -2_665 . -2_565 N
O4 La4 O8 74.6(8) -2_665 . 1_655 N
O4 La4 O8 105.7(8) -2_665 . -1_656 N
O4 La4 O9 173.3(9) -2_665 . 1_555 N
O4 La4 O10 61.2(11) -2_665 . -1_666 N
O6 La4 O8 172.6(10) -2_565 . 1_655 N
O6 La4 O8 98.9(8) -2_565 . -1_656 N
O6 La4 O9 73.9(8) -2_565 . 1_555 N
O6 La4 O10 57.6(13) -2_565 . -1_666 N
O8 La4 O8 78.8(9) 1_655 . -1_656 N
O8 La4 O9 112.0(7) 1_655 . 1_555 N
O8 La4 O10 115.1(14) 1_655 . -1_666 N
O8 La4 O9 75.6(7) -1_656 . 1_555 N
O8 La4 O10 71.1(8) -1_656 . -1_666 N
O9 La4 O10 113.8(13) 1_555 . -1_666 N
Ga2 O1 La1 102.3(10) -2_566 . 1_555 N
Ga2 O1 La2 131.4(12) -2_566 . 1_655 N
Ga2 O1 La4 102.9(10) -2_566 . -2_566 N
Ga2 O1 O4 141.0(12) -2_566 . 1_655 N
Ga2 O1 O5 43.0(8) -2_566 . -2_566 N
Ga2 O1 O7 35.5(7) -2_566 . -2_566 N
Ga2 O1 Ge2 0.0 -2_566 . -2_566 N
Ga2 O1 O10 61.0(14) -2_566 . -1_666 N
La1 O1 La2 104.1(8) 1_555 . 1_655 N
La1 O1 La4 98.9(8) 1_555 . -2_566 N
La1 O1 O4 112.8(9) 1_555 . 1_655 N
La1 O1 O5 60.6(7) 1_555 . -2_566 N
La1 O1 O7 118.1(9) 1_555 . -2_566 N
La1 O1 Ge2 102.3(10) 1_555 . -2_566 N
La1 O1 O10 140.3(13) 1_555 . -1_666 N
La2 O1 La4 112.3(10) 1_655 . -2_566 N
La2 O1 O4 56.0(7) 1_655 . 1_655 N
La2 O1 O5 148.2(11) 1_655 . -2_566 N
La2 O1 O7 137.2(10) 1_655 . -2_566 N
La2 O1 Ge2 131.4(12) 1_655 . -2_566 N
La2 O1 O10 72.7(11) 1_655 . -1_666 N
La4 O1 O4 56.3(8) -2_566 . 1_655 N
La4 O1 O5 98.2(8) -2_566 . -2_566 N
La4 O1 O7 69.4(7) -2_566 . -2_566 N
La4 O1 Ge2 102.9(10) -2_566 . -2_566 N
La4 O1 O10 119.3(12) -2_566 . -1_666 N
O4 O1 O5 153.6(11) 1_655 . -2_566 N
O4 O1 O7 108.8(10) 1_655 . -2_566 N
O4 O1 Ge2 141.0(12) 1_655 . -2_566 N
O4 O1 O10 98.2(13) 1_655 . -1_666 N
O5 O1 O7 61.7(7) -2_566 . -2_566 N
O5 O1 Ge2 43.0(8) -2_566 . -2_566 N
O5 O1 O10 100.8(12) -2_566 . -1_666 N
O7 O1 Ge2 35.5(7) -2_566 . -2_566 N
O7 O1 O10 70.6(11) -2_566 . -1_666 N
Ge2 O1 O10 61.0(14) -2_566 . -1_666 N
Ga1 O2 La1 118.6(9) -2_566 . 1_555 N
Ga1 O2 La2 118.7(10) -2_566 . 1_555 N
Ga1 O2 La3 98.0(9) -2_566 . -2_566 N
Ga1 O2 O3 36.9(7) -2_566 . -2_566 N
Ga1 O2 O5 56.1(8) -2_566 . -2_566 N
Ga1 O2 O7 145.7(10) -2_566 . -1_656 N
Ga1 O2 Ge1 0.0 -2_566 . -2_566 N
Ga1 O2 O10 49.5(10) -2_566 . -1_566 N
La1 O2 La2 109.1(8) 1_555 . 1_555 N
La1 O2 La3 100.2(8) 1_555 . -2_566 N
La1 O2 O3 120.0(8) 1_555 . -2_566 N
La1 O2 O5 63.7(7) 1_555 . -2_566 N
La1 O2 O7 56.1(7) 1_555 . -1_656 N
La1 O2 Ge1 118.6(9) 1_555 . -2_566 N
La1 O2 O10 146.6(12) 1_555 . -1_566 N
La2 O2 La3 109.5(8) 1_555 . -2_566 N
La2 O2 O3 130.8(9) 1_555 . -2_566 N
La2 O2 O5 153.6(9) 1_555 . -2_566 N
La2 O2 O7 52.9(8) 1_555 . -1_656 N
La2 O2 Ge1 118.7(10) 1_555 . -2_566 N
La2 O2 O10 69.4(10) 1_555 . -1_566 N
La3 O2 O3 61.2(5) -2_566 . -2_566 N
La3 O2 O5 96.9(8) -2_566 . -2_566 N
La3 O2 O7 116.2(8) -2_566 . -1_656 N
La3 O2 Ge1 98.0(9) -2_566 . -2_566 N
La3 O2 O10 111.9(12) -2_566 . -1_566 N
O3 O2 O5 63.3(7) -2_566 . -2_566 N
O3 O2 O7 175.5(9) -2_566 . -1_656 N
O3 O2 Ge1 36.9(7) -2_566 . -2_566 N
O3 O2 O10 71.1(9) -2_566 . -1_566 N
O5 O2 O7 114.4(8) -2_566 . -1_656 N
O5 O2 Ge1 56.1(8) -2_566 . -2_566 N
O5 O2 O10 102.2(11) -2_566 . -1_566 N
O7 O2 Ge1 145.7(10) -1_656 . -2_566 N
O7 O2 O10 113.3(12) -1_656 . -1_566 N
Ge1 O2 O10 49.5(10) -2_566 . -1_566 N
Ga1 O3 La1 132.1(11) 1_555 . -1_656 N
Ga1 O3 La2 116.7(11) 1_555 . -1_556 N
Ga1 O3 La3 91.7(7) 1_555 . 1_555 N
Ga1 O3 O2 38.2(7) 1_555 . -2_565 N
Ga1 O3 O5 50.9(8) 1_555 . 1_555 N
Ga1 O3 Ge1 0.0 1_555 . 1_555 N
La1 O3 La2 108.4(6) -1_656 . -1_556 N
La1 O3 La3 95.8(7) -1_656 . 1_555 N
La1 O3 O2 125.3(8) -1_656 . -2_565 N
La1 O3 O5 82.2(8) -1_656 . 1_555 N
La1 O3 Ge1 132.1(11) -1_656 . 1_555 N
La2 O3 La3 100.0(6) -1_556 . 1_555 N
La2 O3 O2 119.8(8) -1_556 . -2_565 N
La2 O3 O5 166.2(8) -1_556 . 1_555 N
La2 O3 Ge1 116.7(11) -1_556 . 1_555 N
La3 O3 O2 53.6(5) 1_555 . -2_565 N
La3 O3 O5 87.3(7) 1_555 . 1_555 N
La3 O3 Ge1 91.7(7) 1_555 . 1_555 N
O2 O3 O5 55.8(7) -2_565 . 1_555 N
O2 O3 Ge1 38.2(7) -2_565 . 1_555 N
O5 O3 Ge1 50.9(8) 1_555 . 1_555 N
Ga1 O4 La2 121.5(13) 1_556 . 1_555 N
Ga1 O4 La3 112.5(11) 1_556 . -2_566 N
Ga1 O4 La4 106.4(10) 1_556 . -2_466 N
Ga1 O4 O1 136.4(12) 1_556 . 1_455 N
Ga1 O4 O5 56.2(9) 1_556 . 1_556 N
Ga1 O4 Ge1 0.0 1_556 . 1_556 N
Ga1 O4 O10 49.2(11) 1_556 . 2_546 N
La2 O4 La3 102.1(8) 1_555 . -2_566 N
La2 O4 La4 109.9(8) 1_555 . -2_466 N
La2 O4 O1 53.3(6) 1_555 . 1_455 N
La2 O4 O5 112.5(10) 1_555 . 1_556 N
La2 O4 Ge1 121.5(13) 1_555 . 1_556 N
La2 O4 O10 123.5(11) 1_555 . 2_546 N
La3 O4 La4 103.1(9) -2_566 . -2_466 N
La3 O4 O1 110.5(8) -2_566 . 1_455 N
La3 O4 O5 60.6(7) -2_566 . 1_556 N
La3 O4 Ge1 112.5(11) -2_566 . 1_556 N
La3 O4 O10 134.2(11) -2_566 . 2_546 N
La4 O4 O1 56.6(7) -2_466 . 1_455 N
La4 O4 O5 136.8(11) -2_466 . 1_556 N
La4 O4 Ge1 106.4(10) -2_466 . 1_556 N
La4 O4 O10 59.5(11) -2_466 . 2_546 N
O1 O4 O5 163.3(11) 1_455 . 1_556 N
O1 O4 Ge1 136.4(12) 1_455 . 1_556 N
O1 O4 O10 94.5(12) 1_455 . 2_546 N
O5 O4 Ge1 56.2(9) 1_556 . 1_556 N
O5 O4 O10 101.5(12) 1_556 . 2_546 N
Ge1 O4 O10 49.2(11) 1_556 . 2_546 N
Ga1 O5 Ga2 161.2(12) 1_555 . 1_555 N
Ga1 O5 La1 96.7(10) 1_555 . -2_565 N
Ga1 O5 La3 96.7(10) 1_555 . -2_565 N
Ga1 O5 O1 147.3(12) 1_555 . -2_565 N
Ga1 O5 O2 42.0(7) 1_555 . -2_565 N
Ga1 O5 O3 37.4(7) 1_555 . 1_555 N
Ga1 O5 O4 40.8(7) 1_555 . 1_554 N
Ga1 O5 O6 140.7(10) 1_555 . 1_554 N
Ga1 O5 O7 125.3(11) 1_555 . 1_555 N
Ga1 O5 Ge1 0.0 1_555 . 1_555 N
Ga1 O5 Ge2 161.2(12) 1_555 . 1_555 N
Ga2 O5 La1 96.8(11) 1_555 . -2_565 N
Ga2 O5 La3 95.1(12) 1_555 . -2_565 N
Ga2 O5 O1 39.2(8) 1_555 . -2_565 N
Ga2 O5 O2 145.7(12) 1_555 . -2_565 N
Ga2 O5 O3 124.6(12) 1_555 . 1_555 N
Ga2 O5 O4 141.0(13) 1_555 . 1_554 N
Ga2 O5 O6 40.9(9) 1_555 . 1_554 N
Ga2 O5 O7 36.1(8) 1_555 . 1_555 N
Ga2 O5 Ge1 161.2(12) 1_555 . 1_555 N
Ga2 O5 Ge2 0.0 1_555 . 1_555 N
La1 O5 La3 95.1(8) -2_565 . -2_565 N
La1 O5 O1 58.8(7) -2_565 . -2_565 N
La1 O5 O2 55.5(6) -2_565 . -2_565 N
La1 O5 O3 110.6(9) -2_565 . 1_555 N
La1 O5 O4 112.8(12) -2_565 . 1_554 N
La1 O5 O6 113.5(10) -2_565 . 1_554 N
La1 O5 O7 115.7(10) -2_565 . 1_555 N
La1 O5 Ge1 96.7(10) -2_565 . 1_555 N
La1 O5 Ge2 96.8(11) -2_565 . 1_555 N
La3 O5 O1 106.1(10) -2_565 . -2_565 N
La3 O5 O2 106.1(10) -2_565 . -2_565 N
La3 O5 O3 127.4(11) -2_565 . 1_555 N
La3 O5 O4 59.0(7) -2_565 . 1_554 N
La3 O5 O6 57.7(8) -2_565 . 1_554 N
La3 O5 O7 121.0(11) -2_565 . 1_555 N
La3 O5 Ge1 96.7(10) -2_565 . 1_555 N
La3 O5 Ge2 95.1(12) -2_565 . 1_555 N
O1 O5 O2 107.7(8) -2_565 . -2_565 N
O1 O5 O3 126.5(10) -2_565 . 1_555 N
O1 O5 O4 163.6(12) -2_565 . 1_554 N
O1 O5 O6 72.0(9) -2_565 . 1_554 N
O1 O5 O7 60.8(8) -2_565 . 1_555 N
O1 O5 Ge1 147.3(12) -2_565 . 1_555 N
O1 O5 Ge2 39.2(8) -2_565 . 1_555 N
O2 O5 O3 60.8(8) -2_565 . 1_555 N
O2 O5 O4 73.1(9) -2_565 . 1_554 N
O2 O5 O6 161.5(10) -2_565 . 1_554 N
O2 O5 O7 132.8(9) -2_565 . 1_555 N
O2 O5 Ge1 42.0(7) -2_565 . 1_555 N
O2 O5 Ge2 145.7(12) -2_565 . 1_555 N
O3 O5 O4 68.7(9) 1_555 . 1_554 N
O3 O5 O6 134.9(10) 1_555 . 1_554 N
O3 O5 O7 88.6(8) 1_555 . 1_555 N
O3 O5 Ge1 37.4(7) 1_555 . 1_555 N
O3 O5 Ge2 124.6(12) 1_555 . 1_555 N
O4 O5 O6 101.9(8) 1_554 . 1_554 N
O4 O5 O7 131.1(11) 1_554 . 1_555 N
O4 O5 Ge1 40.8(7) 1_554 . 1_555 N
O4 O5 Ge2 141.0(13) 1_554 . 1_555 N
O6 O5 O7 64.0(9) 1_554 . 1_555 N
O6 O5 Ge1 140.7(10) 1_554 . 1_555 N
O6 O5 Ge2 40.9(9) 1_554 . 1_555 N
O7 O5 Ge1 125.3(11) 1_555 . 1_555 N
O7 O5 Ge2 36.1(8) 1_555 . 1_555 N
Ge1 O5 Ge2 161.2(12) 1_555 . 1_555 N
Ga2 O6 La1 127.6(16) 1_556 . 1_555 N
Ga2 O6 La3 110.1(12) 1_556 . -2_566 N
Ga2 O6 La4 112.5(14) 1_556 . -2_566 N
Ga2 O6 O5 49.6(10) 1_556 . 1_556 N
Ga2 O6 O7 33.4(9) 1_556 . 1_556 N
Ga2 O6 Ge2 0.0 1_556 . 1_556 N
Ga2 O6 O10 57.8(14) 1_556 . 2_646 N
La1 O6 La3 102.2(10) 1_555 . -2_566 N
La1 O6 La4 101.5(9) 1_555 . -2_566 N
La1 O6 O5 119.1(12) 1_555 . 1_556 N
La1 O6 O7 94.4(10) 1_555 . 1_556 N
La1 O6 Ge2 127.6(16) 1_555 . 1_556 N
La1 O6 O10 120.6(13) 1_555 . 2_646 N
La3 O6 La4 98.9(10) -2_566 . -2_566 N
La3 O6 O5 65.2(8) -2_566 . 1_556 N
La3 O6 O7 128.9(10) -2_566 . 1_556 N
La3 O6 Ge2 110.1(12) -2_566 . 1_556 N
La3 O6 O10 133.5(14) -2_566 . 2_646 N
La4 O6 O5 138.3(11) -2_566 . 1_556 N
La4 O6 O7 124.7(11) -2_566 . 1_556 N
La4 O6 Ge2 112.5(14) -2_566 . 1_556 N
La4 O6 O10 58.0(11) -2_566 . 2_646 N
O5 O6 O7 64.5(8) 1_556 . 1_556 N
O5 O6 Ge2 49.6(10) 1_556 . 1_556 N
O5 O6 O10 103.9(13) 1_556 . 2_646 N
O7 O6 Ge2 33.4(9) 1_556 . 1_556 N
O7 O6 O10 68.3(11) 1_556 . 2_646 N
Ge2 O6 O10 57.8(14) 1_556 . 2_646 N
Ga2 O7 La1 120.7(13) 1_555 . -1_656 N
Ga2 O7 La2 131.6(14) 1_555 . -1_656 N
Ga2 O7 O1 35.8(7) 1_555 . -2_565 N
Ga2 O7 O2 172.6(11) 1_555 . -1_656 N
Ga2 O7 O5 39.8(9) 1_555 . 1_555 N
Ga2 O7 O6 30.9(7) 1_555 . 1_554 N
Ga2 O7 Ge2 0.0 1_555 . 1_555 N
La1 O7 La2 107.1(7) -1_656 . -1_656 N
La1 O7 O1 120.0(9) -1_656 . -2_565 N
La1 O7 O2 55.8(6) -1_656 . -1_656 N
La1 O7 O5 80.9(9) -1_656 . 1_555 N
La1 O7 O6 121.0(10) -1_656 . 1_554 N
La1 O7 Ge2 120.7(13) -1_656 . 1_555 N
La2 O7 O1 113.0(10) -1_656 . -2_565 N
La2 O7 O2 51.2(6) -1_656 . -1_656 N
La2 O7 O5 170.3(11) -1_656 . 1_555 N
La2 O7 O6 124.8(10) -1_656 . 1_554 N
La2 O7 Ge2 131.6(14) -1_656 . 1_555 N
O1 O7 O2 138.3(10) -2_565 . -1_656 N
O1 O7 O5 57.6(8) -2_565 . 1_555 N
O1 O7 O6 65.5(7) -2_565 . 1_554 N
O1 O7 Ge2 35.8(7) -2_565 . 1_555 N
O2 O7 O5 136.5(11) -1_656 . 1_555 N
O2 O7 O6 156.0(8) -1_656 . 1_554 N
O2 O7 Ge2 172.6(11) -1_656 . 1_555 N
O5 O7 O6 51.5(7) 1_555 . 1_554 N
O5 O7 Ge2 39.8(9) 1_555 . 1_555 N
O6 O7 Ge2 30.9(7) 1_554 . 1_555 N
La2 O8 La3 111.8(9) -1_556 . 1_555 N
La2 O8 La4 105.9(9) -1_556 . 1_455 N
La2 O8 La4 119.5(10) -1_556 . -1_656 N
La2 O8 O9 136.2(8) -1_556 . -1_656 N
La2 O8 O10 62.9(9) -1_556 . 1_545 N
La3 O8 La4 110.3(8) 1_555 . 1_455 N
La3 O8 La4 107.4(10) 1_555 . -1_656 N
La3 O8 O9 53.7(7) 1_555 . -1_656 N
La3 O8 O10 126.6(15) 1_555 . 1_545 N
La4 O8 La4 101.2(9) 1_455 . -1_656 N
La4 O8 O9 117.9(7) 1_455 . -1_656 N
La4 O8 O10 122.5(14) 1_455 . 1_545 N
La4 O8 O9 53.7(6) -1_656 . -1_656 N
La4 O8 O10 56.9(9) -1_656 . 1_545 N
O9 O8 O10 91.9(12) -1_656 . 1_545 N
La1 O9 La3 111.6(9) -1_656 . 1_555 N
La1 O9 La3 116.2(9) -1_656 . -1_656 N
La1 O9 La4 112.4(8) -1_656 . 1_555 N
La1 O9 O8 132.3(7) -1_656 . -1_656 N
La3 O9 La3 102.3(7) 1_555 . -1_656 N
La3 O9 La4 110.1(6) 1_555 . 1_555 N
La3 O9 O8 116.1(5) 1_555 . -1_656 N
La3 O9 La4 103.6(8) -1_656 . 1_555 N
La3 O9 O8 53.0(5) -1_656 . -1_656 N
La4 O9 O8 50.7(6) 1_555 . -1_656 N
O2 Ge1 O3 104.8(11) -2_565 . 1_555 N
O2 Ge1 O4 126.3(13) -2_565 . 1_554 N
O2 Ge1 O5 81.9(9) -2_565 . 1_555 N
O2 Ge1 O10 83.7(13) -2_565 . 2_545 N
O3 Ge1 O4 126.9(13) 1_555 . 1_554 N
O3 Ge1 O5 91.7(10) 1_555 . 1_555 N
O3 Ge1 O10 116.0(14) 1_555 . 2_545 N
O4 Ge1 O5 83.0(10) 1_554 . 1_555 N
O4 Ge1 O10 85.8(13) 1_554 . 2_545 N
O5 Ge1 O10 151.2(13) 1_555 . 2_545 N
O1 Ge2 O5 97.8(12) -2_565 . 1_555 N
O1 Ge2 O6 131.5(14) -2_565 . 1_554 N
O1 Ge2 O7 108.8(11) -2_565 . 1_555 N
O1 Ge2 O10 71.6(12) -2_565 . 2_645 N
O5 Ge2 O6 89.5(13) 1_555 . 1_554 N
O5 Ge2 O7 104.0(13) 1_555 . 1_555 N
O5 Ge2 O10 153.7(11) 1_555 . 2_645 N
O6 Ge2 O7 115.8(14) 1_554 . 1_555 N
O6 Ge2 O10 80.9(16) 1_554 . 2_645 N
O7 Ge2 O10 102.2(14) 1_555 . 2_645 N
Ga1 O10 Ga2 143.6(17) 2_555 . 2_655 N
Ga1 O10 La2 98.7(19) 2_555 . -1_566 N
Ga1 O10 La4 102.3(18) 2_555 . -1_666 N
Ga1 O10 O1 132.8(20) 2_555 . -1_666 N
Ga1 O10 O2 46.8(13) 2_555 . -1_566 N
Ga1 O10 O4 45.0(11) 2_555 . 2_556 N
Ga1 O10 O6 139.1(17) 2_555 . 2_656 N
Ga1 O10 O8 110.7(20) 2_555 . 1_565 N
Ga1 O10 Ge1 0.0 2_555 . 2_555 N
Ga1 O10 Ge2 143.6(17) 2_555 . 2_655 N
Ga2 O10 La2 100.3(15) 2_655 . -1_566 N
Ga2 O10 La4 103.1(19) 2_655 . -1_666 N
Ga2 O10 O1 47.3(11) 2_655 . -1_666 N
Ga2 O10 O2 138.2(18) 2_655 . -1_566 N
Ga2 O10 O4 138.9(17) 2_655 . 2_556 N
Ga2 O10 O6 41.3(12) 2_655 . 2_656 N
Ga2 O10 O8 105.4(18) 2_655 . 1_565 N
Ga2 O10 Ge1 143.6(17) 2_655 . 2_555 N
Ga2 O10 Ge2 0.0 2_655 . 2_655 N
La2 O10 La4 103.5(11) -1_566 . -1_666 N
La2 O10 O1 54.2(8) -1_566 . -1_666 N
La2 O10 O2 52.0(9) -1_566 . -1_566 N
La2 O10 O4 119.3(17) -1_566 . 2_556 N
La2 O10 O6 121.7(17) -1_566 . 2_656 N
La2 O10 O8 51.6(7) -1_566 . 1_565 N
La2 O10 Ge1 98.7(19) -1_566 . 2_555 N
La2 O10 Ge2 100.3(15) -1_566 . 2_655 N
La4 O10 O1 120.1(18) -1_666 . -1_666 N
La4 O10 O2 112.9(17) -1_666 . -1_566 N
La4 O10 O4 59.3(10) -1_666 . 2_556 N
La4 O10 O6 64.4(12) -1_666 . 2_656 N
La4 O10 O8 52.1(9) -1_666 . 1_565 N
La4 O10 Ge1 102.3(18) -1_666 . 2_555 N
La4 O10 Ge2 103.1(19) -1_666 . 2_655 N
O1 O10 O2 94.7(13) -1_666 . -1_566 N
O1 O10 O4 173.5(18) -1_666 . 2_556 N
O1 O10 O6 81.9(17) -1_666 . 2_656 N
O1 O10 O8 83.3(11) -1_666 . 1_565 N
O1 O10 Ge1 132.8(20) -1_666 . 2_555 N
O1 O10 Ge2 47.3(11) -1_666 . 2_655 N
O2 O10 O4 80.1(16) -1_566 . 2_556 N
O2 O10 O6 173.1(17) -1_566 . 2_656 N
O2 O10 O8 82.1(12) -1_566 . 1_565 N
O2 O10 Ge1 46.8(13) -1_566 . 2_555 N
O2 O10 Ge2 138.2(18) -1_566 . 2_655 N
O4 O10 O6 102.8(13) 2_556 . 2_656 N
O4 O10 O8 92.0(13) 2_556 . 1_565 N
O4 O10 Ge1 45.0(11) 2_556 . 2_555 N
O4 O10 Ge2 138.9(17) 2_556 . 2_655 N
O6 O10 O8 91.5(16) 2_656 . 1_565 N
O6 O10 Ge1 139.1(17) 2_656 . 2_555 N
O6 O10 Ge2 41.3(12) 2_656 . 2_655 N
O8 O10 Ge1 110.7(20) 1_565 . 2_555 N
O8 O10 Ge2 105.4(18) 1_565 . 2_655 N
Ge1 O10 Ge2 143.6(17) 2_555 . 2_655 N
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ga1 Ga1 5.266(31) . -1_555 N
Ga1 Ga1 5.999(7) . -2_565 N
Ga1 Ga1 5.999(7) . -2_566 N
Ga1 Ga2 3.875(23) . 1_455 N
Ga1 Ga2 4.189(23) . 1_555 N
Ga1 Ga2 5.571(11) . -1_655 N
Ga1 Ga2 5.936(27) . -2_465 N
Ga1 La1 3.933(25) . -1_656 N
Ga1 La1 3.842(22) . -2_565 N
Ga1 La2 3.718(19) . 1_554 N
Ga1 La2 3.681(21) . -1_556 N
Ga1 La2 3.615(20) . -2_565 N
Ga1 La3 3.372(20) . 1_555 N
Ga1 La3 3.792(20) . -2_565 N
Ga1 La4 5.080(19) . 1_455 N
Ga1 La4 4.888(22) . 2_655 N
Ga1 La4 3.480(21) . -2_465 N
Ga1 O1 4.272(24) . 1_454 N
Ga1 O1 4.780(25) . -1_656 N
Ga1 O1 3.907(22) . -2_465 N
Ga1 O1 4.920(22) . -2_565 N
Ga1 O2 4.535(21) . 1_554 N
Ga1 O2 5.913(23) . -1_556 N
Ga1 O2 1.856(22) . -2_565 N
Ga1 O3 1.802(21) . 1_555 N
Ga1 O3 5.840(20) . 2_555 N
Ga1 O3 4.607(20) . -1_555 N
Ga1 O4 1.811(23) . 1_554 N
Ga1 O4 5.123(26) . -1_556 N
Ga1 O4 4.280(22) . -2_565 N
Ga1 O5 5.802(33) . 1_455 N
Ga1 O5 2.303(33) . 1_555 N
Ga1 O5 5.572(28) . -2_566 N
Ga1 O6 4.161(31) . 1_454 N
Ga1 O6 4.573(27) . 1_554 N
Ga1 O6 5.314(31) . -1_656 N
Ga1 O6 4.563(31) . -2_565 N
Ga1 O7 4.122(29) . 1_455 N
Ga1 O7 4.668(28) . 1_555 N
Ga1 O7 4.559(22) . 2_655 N
Ga1 O7 4.545(23) . -1_655 N
Ga1 O8 4.064(25) . 1_555 N
Ga1 O8 3.959(25) . 2_555 N
Ga1 O8 4.246(23) . -2_565 N
Ga1 O9 4.255(21) . 1_555 N
Ga1 O9 4.182(19) . 2_655 N
Ga1 O9 5.715(24) . -1_656 N
Ga1 O9 5.692(21) . -2_465 N
Ga1 Ge1 5.266(31) . -1_555 N
Ga1 Ge1 5.999(7) . -2_565 N
Ga1 Ge1 5.999(7) . -2_566 N
Ga1 Ge2 3.875(23) . 1_455 N
Ga1 Ge2 4.189(23) . 1_555 N
Ga1 Ge2 5.571(11) . -1_655 N
Ga1 Ge2 5.936(27) . -2_465 N
Ga1 O10 5.973(35) . 1_545 N
Ga1 O10 1.94(5) . 2_545 N
Ga1 O10 5.64(4) . -1_565 N
Ga1 O10 5.539(33) . -2_565 N
Ga2 Ga1 4.189(23) . 1_555 N
Ga2 Ga1 3.875(23) . 1_655 N
Ga2 Ga1 5.571(11) . -1_655 N
Ga2 Ga1 5.936(27) . -2_666 N
Ga2 Ga2 5.433(30) . -1_655 N
Ga2 Ga2 5.982(6) . -2_565 N
Ga2 Ga2 5.982(6) . -2_566 N
Ga2 La1 3.775(20) . 1_554 N
Ga2 La1 3.835(23) . -1_656 N
Ga2 La1 3.609(21) . -2_565 N
Ga2 La2 3.818(21) . -1_656 N
Ga2 La2 3.797(19) . -2_665 N
Ga2 La3 4.880(20) . 2_655 N
Ga2 La3 3.510(19) . -2_565 N
Ga2 La4 3.402(20) . 1_555 N
Ga2 La4 3.650(21) . -2_565 N
Ga2 O1 4.683(27) . 1_554 N
Ga2 O1 1.801(25) . -2_565 N
Ga2 O2 4.525(21) . 1_554 N
Ga2 O2 4.682(22) . -1_656 N
Ga2 O2 4.487(22) . -2_565 N
Ga2 O2 4.367(23) . -2_665 N
Ga2 O3 4.374(26) . 1_555 N
Ga2 O3 4.478(25) . 1_655 N
Ga2 O3 4.411(19) . 2_655 N
Ga2 O3 4.769(21) . -1_655 N
Ga2 O3 5.992(21) . -2_565 N
Ga2 O4 4.432(25) . 1_554 N
Ga2 O4 4.398(26) . 1_654 N
Ga2 O4 5.339(29) . -1_656 N
Ga2 O4 4.324(24) . -2_665 N
Ga2 O5 1.943(34) . 1_555 N
Ga2 O5 5.374(26) . -1_655 N
Ga2 O5 5.579(26) . -2_565 N
Ga2 O6 1.669(26) . 1_554 N
Ga2 O6 5.224(31) . -1_656 N
Ga2 O6 4.418(26) . -2_565 N
Ga2 O7 1.788(24) . 1_555 N
Ga2 O7 4.491(28) . -1_655 N
Ga2 O8 4.308(26) . 1_655 N
Ga2 O8 3.982(25) . 2_655 N
Ga2 O8 5.646(26) . -1_656 N
Ga2 O8 5.711(27) . -2_565 N
Ga2 O8 5.941(27) . -2_665 N
Ga2 O9 4.123(24) . 1_555 N
Ga2 O9 3.991(23) . 2_655 N
Ga2 O9 4.204(20) . -2_565 N
Ga2 Ge1 4.189(23) . 1_555 N
Ga2 Ge1 3.875(23) . 1_655 N
Ga2 Ge1 5.571(11) . -1_655 N
Ga2 Ge1 5.936(27) . -2_666 N
Ga2 Ge2 5.433(30) . -1_655 N
Ga2 Ge2 5.982(6) . -2_565 N
Ga2 Ge2 5.982(6) . -2_566 N
Ga2 O10 2.14(5) . 2_645 N
Ga2 O10 5.42(4) . -1_666 N
La1 Ga1 3.933(25) . -1_656 N
La1 Ga1 3.842(22) . -2_566 N
La1 Ga2 3.775(20) . 1_556 N
La1 Ga2 3.835(23) . -1_656 N
La1 Ga2 3.609(21) . -2_566 N
La1 La2 4.015(24) . 1_555 N
La1 La2 4.051(24) . 1_655 N
La1 La3 4.114(22) . 1_555 N
La1 La3 3.928(18) . -1_656 N
La1 La3 3.957(23) . -2_566 N
La1 La4 4.006(20) . -1_656 N
La1 La4 4.017(25) . -2_566 N
La1 O1 2.769(26) . 1_555 N
La1 O1 4.781(26) . 2_646 N
La1 O2 2.591(22) . 1_555 N
La1 O2 4.790(22) . 2_646 N
La1 O3 2.491(24) . -1_656 N
La1 O3 4.758(24) . -2_566 N
La1 O4 4.826(28) . 1_555 N
La1 O4 4.616(26) . 1_655 N
La1 O4 4.930(27) . -1_657 N
La1 O4 4.639(27) . -2_565 N
La1 O5 4.369(27) . 1_556 N
La1 O5 3.606(25) . -1_656 N
La1 O5 2.819(24) . -2_566 N
La1 O6 2.517(25) . 1_555 N
La1 O6 5.022(29) . 2_646 N
La1 O6 4.815(31) . -1_657 N
La1 O6 4.493(27) . -2_565 N
La1 O7 4.007(22) . 1_556 N
La1 O7 2.600(31) . -1_656 N
La1 O7 4.878(23) . -2_566 N
La1 O8 4.868(29) . 1_555 N
La1 O8 4.797(27) . -1_556 N
La1 O8 4.582(28) . -1_656 N
La1 O9 4.926(22) . 1_555 N
La1 O9 2.357(23) . -1_656 N
La1 O9 4.634(26) . -2_566 N
La1 Ge1 3.933(25) . -1_656 N
La1 Ge1 3.842(22) . -2_566 N
La1 Ge2 3.775(20) . 1_556 N
La1 Ge2 3.835(23) . -1_656 N
La1 Ge2 3.609(21) . -2_566 N
La1 O10 4.36(4) . 2_646 N
La1 O10 4.91(5) . -1_566 N
La1 O10 4.79(5) . -1_666 N
La2 Ga1 3.718(19) . 1_556 N
La2 Ga1 3.681(21) . -1_556 N
La2 Ga1 3.615(20) . -2_566 N
La2 Ga2 3.818(21) . -1_656 N
La2 Ga2 3.797(19) . -2_466 N
La2 La1 4.051(24) . 1_455 N
La2 La1 4.015(24) . 1_555 N
La2 La3 4.062(19) . -1_556 N
La2 La3 4.006(23) . -2_566 N
La2 La4 4.152(19) . 1_455 N
La2 La4 3.957(17) . -1_656 N
La2 La4 4.045(19) . -2_466 N
La2 O1 2.357(23) . 1_455 N
La2 O1 4.434(23) . 2_646 N
La2 O2 2.335(25) . 1_555 N
La2 O2 4.677(26) . 2_546 N
La2 O3 4.226(18) . 1_556 N
La2 O3 2.502(25) . -1_556 N
La2 O3 4.766(21) . -2_566 N
La2 O4 2.437(24) . 1_555 N
La2 O4 4.915(24) . 2_546 N
La2 O4 4.820(27) . -1_557 N
La2 O4 4.597(24) . -2_565 N
La2 O5 4.317(28) . 1_556 N
La2 O5 4.983(30) . -2_466 N
La2 O5 4.947(33) . -2_566 N
La2 O6 4.788(29) . 1_455 N
La2 O6 4.692(33) . 1_555 N
La2 O6 4.719(29) . -1_657 N
La2 O6 4.607(31) . -2_465 N
La2 O7 2.389(26) . -1_656 N
La2 O7 4.915(25) . -2_466 N
La2 O8 4.962(25) . 1_555 N
La2 O8 2.441(25) . -1_556 N
La2 O8 4.721(27) . -2_566 N
La2 O9 5.014(22) . 1_455 N
La2 O9 4.732(23) . -1_556 N
La2 O9 4.651(25) . -1_656 N
La2 Ge1 3.718(19) . 1_556 N
La2 Ge1 3.681(21) . -1_556 N
La2 Ge1 3.615(20) . -2_566 N
La2 Ge2 3.818(21) . -1_656 N
La2 Ge2 3.797(19) . -2_466 N
La2 O10 4.39(4) . 2_546 N
La2 O10 2.774(32) . -1_566 N
La2 O10 3.842(35) . -2_566 N
La3 Ga1 3.372(20) . 1_555 N
La3 Ga1 3.792(20) . -2_566 N
La3 Ga2 4.880(20) . 2_645 N
La3 Ga2 3.510(19) . -2_566 N
La3 La1 4.114(22) . 1_555 N
La3 La1 3.928(18) . -1_656 N
La3 La1 3.957(23) . -2_565 N
La3 La2 4.062(19) . -1_556 N
La3 La2 4.006(23) . -2_565 N
La3 La3 3.800(27) . -1_656 N
La3 La4 4.086(20) . 1_455 N
La3 La4 3.979(21) . 1_555 N
La3 La4 3.892(14) . -1_656 N
La3 O1 4.458(21) . 1_555 N
La3 O1 4.421(26) . -1_656 N
La3 O1 4.507(24) . -2_465 N
La3 O1 4.929(24) . -2_565 N
La3 O2 4.398(23) . 1_555 N
La3 O2 2.568(23) . -2_565 N
La3 O3 2.796(17) . 1_555 N
La3 O4 2.710(23) . -2_565 N
La3 O5 3.979(30) . 1_555 N
La3 O5 4.939(26) . 2_645 N
La3 O5 2.756(27) . -2_566 N
La3 O6 4.572(31) . 2_646 N
La3 O6 2.566(30) . -2_565 N
La3 O7 5.073(24) . 1_555 N
La3 O7 4.649(23) . 2_655 N
La3 O7 4.961(23) . -2_566 N
La3 O8 2.464(27) . 1_555 N
La3 O8 4.843(23) . -1_556 N
La3 O8 4.551(24) . -1_656 N
La3 O9 2.392(21) . 1_555 N
La3 O9 2.488(22) . -1_656 N
La3 Ge1 3.372(20) . 1_555 N
La3 Ge1 3.792(20) . -2_566 N
La3 Ge2 4.880(20) . 2_645 N
La3 Ge2 3.510(19) . -2_566 N
La3 O10 4.74(4) . 1_545 N
La3 O10 4.22(5) . 2_545 N
La3 O10 4.85(5) . -1_566 N
La3 O10 4.65(5) . -1_666 N
La4 Ga1 5.080(19) . 1_655 N
La4 Ga1 4.888(22) . 2_645 N
La4 Ga1 3.480(21) . -2_666 N
La4 Ga2 3.402(20) . 1_555 N
La4 Ga2 3.650(21) . -2_566 N
La4 La1 4.006(20) . -1_656 N
La4 La1 4.017(25) . -2_565 N
La4 La2 4.152(19) . 1_655 N
La4 La2 3.957(17) . -1_656 N
La4 La2 4.045(19) . -2_665 N
La4 La3 3.979(21) . 1_555 N
La4 La3 4.086(20) . 1_655 N
La4 La3 3.892(14) . -1_656 N
La4 La4 3.771(31) . -1_756 N
La4 O1 4.189(27) . 1_555 N
La4 O1 2.513(27) . -2_565 N
La4 O2 4.200(21) . 1_655 N
La4 O2 4.249(23) . -1_656 N
La4 O2 4.939(23) . -2_565 N
La4 O2 4.665(21) . -2_665 N
La4 O3 4.947(24) . 1_555 N
La4 O3 4.882(21) . 1_655 N
La4 O3 4.802(20) . 2_655 N
La4 O3 5.073(19) . -1_656 N
La4 O4 4.511(27) . 2_646 N
La4 O4 2.504(27) . -2_665 N
La4 O5 4.037(30) . 1_555 N
La4 O5 4.971(30) . 2_645 N
La4 O5 4.880(33) . -2_566 N
La4 O5 4.886(32) . -2_666 N
La4 O6 5.069(27) . 1_554 N
La4 O6 2.670(31) . -2_565 N
La4 O7 3.109(20) . 1_555 N
La4 O7 4.960(24) . -2_566 N
La4 O8 2.515(26) . 1_655 N
La4 O8 2.363(25) . -1_656 N
La4 O9 2.463(23) . 1_555 N
La4 O9 4.731(23) . -1_656 N
La4 O9 4.694(25) . -1_756 N
La4 Ge1 5.080(19) . 1_655 N
La4 Ge1 4.888(22) . 2_645 N
La4 Ge1 3.480(21) . -2_666 N
La4 Ge2 3.402(20) . 1_555 N
La4 Ge2 3.650(21) . -2_566 N
La4 O10 4.69(4) . 1_645 N
La4 O10 4.17(4) . 2_645 N
La4 O10 2.51(4) . -1_666 N
O1 Ga1 4.272(24) . 1_656 N
O1 Ga1 4.780(25) . -1_656 N
O1 Ga1 4.920(22) . -2_566 N
O1 Ga1 3.907(22) . -2_666 N
O1 Ga2 4.683(27) . 1_556 N
O1 Ga2 1.801(25) . -2_566 N
O1 La1 2.769(26) . 1_555 N
O1 La1 4.781(26) . 2_656 N
O1 La2 2.357(23) . 1_655 N
O1 La2 4.434(23) . 2_656 N
O1 La3 4.458(21) . 1_555 N
O1 La3 4.421(26) . -1_656 N
O1 La3 4.929(24) . -2_566 N
O1 La3 4.507(24) . -2_666 N
O1 La4 4.189(27) . 1_555 N
O1 La4 2.513(27) . -2_566 N
O1 O1 5.876(4) . -2_565 N
O1 O1 5.876(4) . -2_566 N
O1 O2 4.497(19) . 1_555 N
O1 O2 3.572(19) . 1_655 N
O1 O2 5.733(35) . 2_646 N
O1 O2 5.44(4) . 2_656 N
O1 O2 5.739(34) . -2_666 N
O1 O3 5.356(25) . 1_656 N
O1 O3 3.023(23) . -1_656 N
O1 O3 5.170(28) . -2_566 N
O1 O3 4.609(27) . -2_666 N
O1 O4 2.774(26) . 1_655 N
O1 O4 5.932(32) . -1_657 N
O1 O4 5.514(26) . -2_565 N
O1 O4 4.868(26) . -2_665 N
O1 O5 5.886(34) . 1_556 N
O1 O5 5.46(4) . 1_656 N
O1 O5 5.654(32) . -1_656 N
O1 O5 2.82(4) . -2_566 N
O1 O5 5.97(4) . -2_666 N
O1 O6 3.346(33) . 1_555 N
O1 O6 3.164(32) . -2_565 N
O1 O7 5.341(28) . 1_556 N
O1 O7 5.367(29) . -1_656 N
O1 O7 4.742(30) . -1_756 N
O1 O7 2.917(26) . -2_566 N
O1 O8 4.866(29) . 2_656 N
O1 O8 3.451(30) . -1_656 N
O1 O8 3.880(31) . -2_666 N
O1 O9 4.697(26) . 1_555 N
O1 O9 3.851(26) . -1_656 N
O1 O9 4.109(25) . -2_566 N
O1 Ge1 4.272(24) . 1_656 N
O1 Ge1 4.780(25) . -1_656 N
O1 Ge1 4.920(22) . -2_566 N
O1 Ge1 3.907(22) . -2_666 N
O1 Ge2 4.683(27) . 1_556 N
O1 Ge2 1.801(25) . -2_566 N
O1 O10 3.91(4) . 2_646 N
O1 O10 2.32(4) . -1_666 N
O1 O10 5.70(4) . -2_666 N
O2 Ga1 4.535(21) . 1_556 N
O2 Ga1 5.913(23) . -1_556 N
O2 Ga1 1.856(22) . -2_566 N
O2 Ga2 4.525(21) . 1_556 N
O2 Ga2 4.682(22) . -1_656 N
O2 Ga2 4.367(23) . -2_466 N
O2 Ga2 4.487(22) . -2_566 N
O2 La1 2.591(22) . 1_555 N
O2 La1 4.790(22) . 2_656 N
O2 La2 2.335(25) . 1_555 N
O2 La2 4.677(26) . 2_556 N
O2 La3 4.398(23) . 1_555 N
O2 La3 2.568(23) . -2_566 N
O2 La4 4.200(21) . 1_455 N
O2 La4 4.249(23) . -1_656 N
O2 La4 4.665(21) . -2_466 N
O2 La4 4.939(23) . -2_566 N
O2 O1 3.572(19) . 1_455 N
O2 O1 4.497(19) . 1_555 N
O2 O1 5.44(4) . 2_646 N
O2 O1 5.733(35) . 2_656 N
O2 O1 5.739(34) . -2_465 N
O2 O2 5.914(5) . -2_565 N
O2 O2 5.914(5) . -2_566 N
O2 O3 5.386(22) . 1_556 N
O2 O3 4.822(26) . -1_556 N
O2 O3 5.074(27) . -1_656 N
O2 O3 2.899(22) . -2_566 N
O2 O4 3.021(26) . 1_555 N
O2 O4 3.271(26) . -2_565 N
O2 O5 4.007(27) . 1_556 N
O2 O5 5.429(27) . -1_656 N
O2 O5 2.746(34) . -2_566 N
O2 O6 3.226(33) . 1_555 N
O2 O6 5.705(32) . -1_657 N
O2 O6 5.021(34) . -2_465 N
O2 O6 5.229(28) . -2_565 N
O2 O7 5.274(26) . 1_556 N
O2 O7 2.904(24) . -1_656 N
O2 O7 4.885(32) . -2_466 N
O2 O7 5.214(29) . -2_566 N
O2 O8 4.574(26) . 1_555 N
O2 O8 3.532(27) . -1_556 N
O2 O8 4.003(25) . -2_566 N
O2 O9 5.034(25) . 2_656 N
O2 O9 3.640(22) . -1_656 N
O2 O9 4.120(22) . -2_566 N
O2 Ge1 4.535(21) . 1_556 N
O2 Ge1 5.913(23) . -1_556 N
O2 Ge1 1.856(22) . -2_566 N
O2 Ge2 4.525(21) . 1_556 N
O2 Ge2 4.682(22) . -1_656 N
O2 Ge2 4.367(23) . -2_466 N
O2 Ge2 4.487(22) . -2_566 N
O2 O10 5.55(5) . 2_546 N
O2 O10 5.70(5) . 2_646 N
O2 O10 2.53(5) . -1_566 N
O2 O10 5.60(4) . -2_566 N
O3 Ga1 1.802(21) . 1_555 N
O3 Ga1 5.840(20) . 2_545 N
O3 Ga1 4.607(20) . -1_555 N
O3 Ga2 4.478(25) . 1_455 N
O3 Ga2 4.374(26) . 1_555 N
O3 Ga2 4.411(19) . 2_645 N
O3 Ga2 4.769(21) . -1_655 N
O3 Ga2 5.992(21) . -2_566 N
O3 La1 2.491(24) . -1_656 N
O3 La1 4.758(24) . -2_565 N
O3 La2 4.226(18) . 1_554 N
O3 La2 2.502(25) . -1_556 N
O3 La2 4.766(21) . -2_565 N
O3 La3 2.796(17) . 1_555 N
O3 La4 4.882(21) . 1_455 N
O3 La4 4.947(24) . 1_555 N
O3 La4 4.802(20) . 2_645 N
O3 La4 5.073(19) . -1_656 N
O3 O1 5.356(25) . 1_454 N
O3 O1 3.023(23) . -1_656 N
O3 O1 4.609(27) . -2_465 N
O3 O1 5.170(28) . -2_565 N
O3 O2 5.386(22) . 1_554 N
O3 O2 4.822(26) . -1_556 N
O3 O2 5.074(27) . -1_656 N
O3 O2 2.899(22) . -2_565 N
O3 O3 4.605(30) . -1_555 N
O3 O4 3.232(23) . 1_554 N
O3 O4 3.977(28) . -1_556 N
O3 O4 4.492(24) . -2_565 N
O3 O5 2.967(31) . 1_555 N
O3 O5 4.591(29) . 2_645 N
O3 O5 5.489(28) . -2_566 N
O3 O6 5.083(35) . 1_454 N
O3 O6 5.098(33) . 1_554 N
O3 O6 5.080(28) . 2_646 N
O3 O6 4.055(28) . -1_656 N
O3 O6 4.574(33) . -2_565 N
O3 O7 3.961(31) . 1_455 N
O3 O7 4.126(30) . 1_555 N
O3 O7 5.886(29) . 2_645 N
O3 O7 5.798(28) . 2_655 N
O3 O7 4.325(22) . -1_655 N
O3 O8 3.074(26) . 1_555 N
O3 O8 5.623(24) . 2_555 N
O3 O8 5.989(24) . -2_565 N
O3 O9 3.097(23) . 1_555 N
O3 O9 5.634(21) . 2_655 N
O3 O9 4.642(22) . -1_656 N
O3 Ge1 1.802(21) . 1_555 N
O3 Ge1 5.840(20) . 2_545 N
O3 Ge1 4.607(20) . -1_555 N
O3 Ge2 4.478(25) . 1_455 N
O3 Ge2 4.374(26) . 1_555 N
O3 Ge2 4.411(19) . 2_645 N
O3 Ge2 4.769(21) . -1_655 N
O3 Ge2 5.992(21) . -2_566 N
O3 O10 4.410(35) . 1_545 N
O3 O10 3.17(5) . 2_545 N
O3 O10 4.594(33) . -2_565 N
O4 Ga1 1.811(23) . 1_556 N
O4 Ga1 5.123(26) . -1_556 N
O4 Ga1 4.280(22) . -2_566 N
O4 Ga2 4.398(26) . 1_456 N
O4 Ga2 4.432(25) . 1_556 N
O4 Ga2 5.339(29) . -1_656 N
O4 Ga2 4.324(24) . -2_466 N
O4 La1 4.616(26) . 1_455 N
O4 La1 4.826(28) . 1_555 N
O4 La1 4.930(27) . -1_657 N
O4 La1 4.639(27) . -2_566 N
O4 La2 2.437(24) . 1_555 N
O4 La2 4.915(24) . 2_556 N
O4 La2 4.820(27) . -1_557 N
O4 La2 4.597(24) . -2_566 N
O4 La3 2.710(23) . -2_566 N
O4 La4 4.511(27) . 2_656 N
O4 La4 2.504(27) . -2_466 N
O4 O1 2.774(26) . 1_455 N
O4 O1 5.932(32) . -1_657 N
O4 O1 4.868(26) . -2_466 N
O4 O1 5.514(26) . -2_566 N
O4 O2 3.021(26) . 1_555 N
O4 O2 3.271(26) . -2_566 N
O4 O3 3.232(23) . 1_556 N
O4 O3 3.977(28) . -1_556 N
O4 O3 4.492(24) . -2_566 N
O4 O4 5.60(5) . -1_557 N
O4 O4 5.8557(29) . -2_565 N
O4 O4 5.8557(29) . -2_566 N
O4 O5 2.75(4) . 1_556 N
O4 O5 5.45(4) . -2_466 N
O4 O5 5.62(4) . -2_566 N
O4 O6 3.949(34) . 1_455 N
O4 O6 4.119(34) . 1_555 N
O4 O6 5.634(17) . -1_657 N
O4 O6 5.72(4) . -2_465 N
O4 O7 4.928(31) . 1_456 N
O4 O7 5.182(30) . 1_556 N
O4 O7 5.335(26) . 2_656 N
O4 O7 3.893(29) . -1_656 N
O4 O7 4.629(31) . -2_466 N
O4 O8 5.736(28) . 1_556 N
O4 O8 3.880(27) . 2_556 N
O4 O8 4.805(29) . -1_556 N
O4 O8 3.042(35) . -2_566 N
O4 O9 5.756(27) . 1_556 N
O4 O9 3.988(28) . 2_656 N
O4 O9 4.959(26) . -2_466 N
O4 O9 5.102(25) . -2_566 N
O4 Ge1 1.811(23) . 1_556 N
O4 Ge1 5.123(26) . -1_556 N
O4 Ge1 4.280(22) . -2_566 N
O4 Ge2 4.398(26) . 1_456 N
O4 Ge2 4.432(25) . 1_556 N
O4 Ge2 5.339(29) . -1_656 N
O4 Ge2 4.324(24) . -2_466 N
O4 O10 2.55(4) . 2_546 N
O4 O10 3.866(34) . -1_566 N
O4 O10 5.45(4) . -2_566 N
O4 O10 5.85(4) . -2_576 N
O5 Ga1 2.303(33) . 1_555 N
O5 Ga1 5.802(33) . 1_655 N
O5 Ga1 5.572(28) . -2_565 N
O5 Ga2 1.943(34) . 1_555 N
O5 Ga2 5.374(26) . -1_655 N
O5 Ga2 5.579(26) . -2_566 N
O5 La1 4.369(27) . 1_554 N
O5 La1 3.606(25) . -1_656 N
O5 La1 2.819(24) . -2_565 N
O5 La2 4.317(28) . 1_554 N
O5 La2 4.947(33) . -2_565 N
O5 La2 4.983(30) . -2_665 N
O5 La3 3.979(30) . 1_555 N
O5 La3 4.939(26) . 2_655 N
O5 La3 2.756(27) . -2_565 N
O5 La4 4.037(30) . 1_555 N
O5 La4 4.971(30) . 2_655 N
O5 La4 4.886(32) . -2_465 N
O5 La4 4.880(33) . -2_565 N
O5 O1 5.46(4) . 1_454 N
O5 O1 5.886(34) . 1_554 N
O5 O1 5.654(32) . -1_656 N
O5 O1 5.97(4) . -2_465 N
O5 O1 2.82(4) . -2_565 N
O5 O2 4.007(27) . 1_554 N
O5 O2 5.429(27) . -1_656 N
O5 O2 2.746(34) . -2_565 N
O5 O3 2.967(31) . 1_555 N
O5 O3 4.591(29) . 2_655 N
O5 O3 5.489(28) . -2_565 N
O5 O4 2.75(4) . 1_554 N
O5 O4 5.62(4) . -2_565 N
O5 O4 5.45(4) . -2_665 N
O5 O5 5.98(5) . -1_655 N
O5 O5 5.878(5) . -2_565 N
O5 O5 5.878(5) . -2_566 N
O5 O6 2.551(31) . 1_554 N
O5 O6 5.17(4) . -1_656 N
O5 O6 3.918(25) . -2_565 N
O5 O7 2.942(34) . 1_555 N
O5 O7 4.749(32) . 2_655 N
O5 O7 4.225(29) . -1_655 N
O5 O8 5.578(34) . 1_555 N
O5 O8 5.67(4) . 1_655 N
O5 O8 5.194(34) . 2_555 N
O5 O8 5.00(4) . 2_655 N
O5 O8 4.393(32) . -2_565 N
O5 O9 3.842(28) . 1_555 N
O5 O9 3.161(26) . 2_655 N
O5 O9 4.412(30) . -2_565 N
O5 Ge1 2.303(33) . 1_555 N
O5 Ge1 5.802(33) . 1_655 N
O5 Ge1 5.572(28) . -2_565 N
O5 Ge2 1.943(34) . 1_555 N
O5 Ge2 5.374(26) . -1_655 N
O5 Ge2 5.579(26) . -2_566 N
O5 O10 4.11(6) . 2_545 N
O5 O10 3.98(6) . 2_645 N
O5 O10 5.97(6) . -1_565 N
O5 O10 5.74(6) . -1_666 N
O6 Ga1 4.573(27) . 1_556 N
O6 Ga1 4.161(31) . 1_656 N
O6 Ga1 5.314(31) . -1_656 N
O6 Ga1 4.563(31) . -2_566 N
O6 Ga2 1.669(26) . 1_556 N
O6 Ga2 5.224(31) . -1_656 N
O6 Ga2 4.418(26) . -2_566 N
O6 La1 2.517(25) . 1_555 N
O6 La1 5.022(29) . 2_656 N
O6 La1 4.815(31) . -1_657 N
O6 La1 4.493(27) . -2_566 N
O6 La2 4.692(33) . 1_555 N
O6 La2 4.788(29) . 1_655 N
O6 La2 4.719(29) . -1_657 N
O6 La2 4.607(31) . -2_666 N
O6 La3 4.572(31) . 2_656 N
O6 La3 2.566(30) . -2_566 N
O6 La4 5.069(27) . 1_556 N
O6 La4 2.670(31) . -2_566 N
O6 O1 3.346(33) . 1_555 N
O6 O1 3.164(32) . -2_566 N
O6 O2 3.226(33) . 1_555 N
O6 O2 5.705(32) . -1_657 N
O6 O2 5.229(28) . -2_566 N
O6 O2 5.021(34) . -2_666 N
O6 O3 5.098(33) . 1_556 N
O6 O3 5.083(35) . 1_656 N
O6 O3 5.080(28) . 2_656 N
O6 O3 4.055(28) . -1_656 N
O6 O3 4.574(33) . -2_566 N
O6 O4 4.119(34) . 1_555 N
O6 O4 3.949(34) . 1_655 N
O6 O4 5.634(17) . -1_657 N
O6 O4 5.72(4) . -2_666 N
O6 O5 2.551(31) . 1_556 N
O6 O5 5.17(4) . -1_656 N
O6 O5 3.918(25) . -2_566 N
O6 O6 5.53(6) . -1_657 N
O6 O6 5.862(4) . -2_565 N
O6 O6 5.862(4) . -2_566 N
O6 O7 2.929(28) . 1_556 N
O6 O7 3.92(4) . -1_656 N
O6 O7 4.841(28) . -2_566 N
O6 O8 5.712(34) . 1_656 N
O6 O8 3.83(4) . 2_656 N
O6 O8 5.017(33) . -2_566 N
O6 O8 5.174(32) . -2_666 N
O6 O9 5.601(30) . 1_556 N
O6 O9 3.928(28) . 2_656 N
O6 O9 4.851(27) . -1_656 N
O6 O9 3.088(35) . -2_566 N
O6 Ge1 4.573(27) . 1_556 N
O6 Ge1 4.161(31) . 1_656 N
O6 Ge1 5.314(31) . -1_656 N
O6 Ge1 4.563(31) . -2_566 N
O6 Ge2 1.669(26) . 1_556 N
O6 Ge2 5.224(31) . -1_656 N
O6 Ge2 4.418(26) . -2_566 N
O6 O10 2.50(6) . 2_646 N
O6 O10 5.69(6) . -1_566 N
O6 O10 5.65(5) . -1_666 N
O7 Ga1 4.668(28) . 1_555 N
O7 Ga1 4.122(29) . 1_655 N
O7 Ga1 4.559(22) . 2_645 N
O7 Ga1 4.545(23) . -1_655 N
O7 Ga2 1.788(24) . 1_555 N
O7 Ga2 4.491(28) . -1_655 N
O7 La1 4.007(22) . 1_554 N
O7 La1 2.600(31) . -1_656 N
O7 La1 4.878(23) . -2_565 N
O7 La2 2.389(26) . -1_656 N
O7 La2 4.915(25) . -2_665 N
O7 La3 5.073(24) . 1_555 N
O7 La3 4.649(23) . 2_645 N
O7 La3 4.961(23) . -2_565 N
O7 La4 3.109(20) . 1_555 N
O7 La4 4.960(24) . -2_565 N
O7 O1 5.341(28) . 1_554 N
O7 O1 5.367(29) . -1_656 N
O7 O1 4.742(30) . -1_756 N
O7 O1 2.917(26) . -2_565 N
O7 O2 5.274(26) . 1_554 N
O7 O2 2.904(24) . -1_656 N
O7 O2 5.214(29) . -2_565 N
O7 O2 4.885(32) . -2_665 N
O7 O3 4.126(30) . 1_555 N
O7 O3 3.961(31) . 1_655 N
O7 O3 5.798(28) . 2_645 N
O7 O3 5.886(29) . 2_655 N
O7 O3 4.325(22) . -1_655 N
O7 O4 5.182(30) . 1_554 N
O7 O4 4.928(31) . 1_654 N
O7 O4 5.335(26) . 2_646 N
O7 O4 3.893(29) . -1_656 N
O7 O4 4.629(31) . -2_665 N
O7 O5 2.942(34) . 1_555 N
O7 O5 4.749(32) . 2_645 N
O7 O5 4.225(29) . -1_655 N
O7 O6 2.929(28) . 1_554 N
O7 O6 3.92(4) . -1_656 N
O7 O6 4.841(28) . -2_565 N
O7 O7 4.15(4) . -1_655 N
O7 O8 3.385(31) . 1_655 N
O7 O8 5.539(29) . 2_655 N
O7 O8 4.871(26) . -1_656 N
O7 O9 3.357(28) . 1_555 N
O7 O9 5.654(24) . 2_655 N
O7 O9 5.868(23) . -2_565 N
O7 Ge1 4.668(28) . 1_555 N
O7 Ge1 4.122(29) . 1_655 N
O7 Ge1 4.559(22) . 2_645 N
O7 Ge1 4.545(23) . -1_655 N
O7 Ge2 1.788(24) . 1_555 N
O7 Ge2 4.491(28) . -1_655 N
O7 O10 4.54(4) . 1_645 N
O7 O10 3.07(4) . 2_645 N
O7 O10 5.56(4) . -1_666 N
O7 O10 5.95(5) . -2_565 N
O7 O10 5.91(4) . -2_665 N
O8 Ga1 4.064(25) . 1_555 N
O8 Ga1 3.959(25) . 2_545 N
O8 Ga1 4.246(23) . -2_566 N
O8 Ga2 4.308(26) . 1_455 N
O8 Ga2 3.982(25) . 2_645 N
O8 Ga2 5.646(26) . -1_656 N
O8 Ga2 5.941(27) . -2_466 N
O8 Ga2 5.711(27) . -2_566 N
O8 La1 4.868(29) . 1_555 N
O8 La1 4.797(27) . -1_556 N
O8 La1 4.582(28) . -1_656 N
O8 La2 4.962(25) . 1_555 N
O8 La2 2.441(25) . -1_556 N
O8 La2 4.721(27) . -2_565 N
O8 La3 2.464(27) . 1_555 N
O8 La3 4.843(23) . -1_556 N
O8 La3 4.551(24) . -1_656 N
O8 La4 2.515(26) . 1_455 N
O8 La4 2.363(25) . -1_656 N
O8 O1 4.866(29) . 2_646 N
O8 O1 3.451(30) . -1_656 N
O8 O1 3.880(31) . -2_465 N
O8 O2 4.574(26) . 1_555 N
O8 O2 3.532(27) . -1_556 N
O8 O2 4.003(25) . -2_565 N
O8 O3 3.074(26) . 1_555 N
O8 O3 5.623(24) . 2_545 N
O8 O3 5.989(24) . -2_566 N
O8 O4 5.736(28) . 1_554 N
O8 O4 3.880(27) . 2_546 N
O8 O4 4.805(29) . -1_556 N
O8 O4 3.042(35) . -2_565 N
O8 O5 5.67(4) . 1_455 N
O8 O5 5.578(34) . 1_555 N
O8 O5 5.194(34) . 2_545 N
O8 O5 5.00(4) . 2_645 N
O8 O5 4.393(32) . -2_566 N
O8 O6 5.712(34) . 1_454 N
O8 O6 3.83(4) . 2_646 N
O8 O6 5.174(32) . -2_465 N
O8 O6 5.017(33) . -2_565 N
O8 O7 3.385(31) . 1_455 N
O8 O7 5.539(29) . 2_645 N
O8 O7 4.871(26) . -1_656 N
O8 O8 3.10(4) . -1_556 N
O8 O9 4.128(31) . 1_455 N
O8 O9 3.937(31) . 1_555 N
O8 O9 2.958(19) . -1_656 N
O8 Ge1 4.064(25) . 1_555 N
O8 Ge1 3.959(25) . 2_545 N
O8 Ge1 4.246(23) . -2_566 N
O8 Ge2 4.308(26) . 1_455 N
O8 Ge2 3.982(25) . 2_645 N
O8 Ge2 5.646(26) . -1_656 N
O8 Ge2 5.941(27) . -2_466 N
O8 Ge2 5.711(27) . -2_566 N
O8 O10 2.835(34) . 1_545 N
O8 O10 4.18(4) . 2_545 N
O8 O10 4.24(5) . -1_566 N
O9 Ga1 4.255(21) . 1_555 N
O9 Ga1 4.182(19) . 2_645 N
O9 Ga1 5.715(24) . -1_656 N
O9 Ga1 5.692(21) . -2_666 N
O9 Ga2 4.123(24) . 1_555 N
O9 Ga2 3.991(23) . 2_645 N
O9 Ga2 4.204(20) . -2_566 N
O9 La1 4.926(22) . 1_555 N
O9 La1 2.357(23) . -1_656 N
O9 La1 4.634(26) . -2_565 N
O9 La2 5.014(22) . 1_655 N
O9 La2 4.732(23) . -1_556 N
O9 La2 4.651(25) . -1_656 N
O9 La3 2.392(21) . 1_555 N
O9 La3 2.488(22) . -1_656 N
O9 La4 2.463(23) . 1_555 N
O9 La4 4.731(23) . -1_656 N
O9 La4 4.694(25) . -1_756 N
O9 O1 4.697(26) . 1_555 N
O9 O1 3.851(26) . -1_656 N
O9 O1 4.109(25) . -2_565 N
O9 O2 5.034(25) . 2_646 N
O9 O2 3.640(22) . -1_656 N
O9 O2 4.120(22) . -2_565 N
O9 O3 3.097(23) . 1_555 N
O9 O3 5.634(21) . 2_645 N
O9 O3 4.642(22) . -1_656 N
O9 O4 5.756(27) . 1_554 N
O9 O4 3.988(28) . 2_646 N
O9 O4 5.102(25) . -2_565 N
O9 O4 4.959(26) . -2_665 N
O9 O5 3.842(28) . 1_555 N
O9 O5 3.161(26) . 2_645 N
O9 O5 4.412(30) . -2_566 N
O9 O6 5.601(30) . 1_554 N
O9 O6 3.928(28) . 2_646 N
O9 O6 4.851(27) . -1_656 N
O9 O6 3.088(35) . -2_565 N
O9 O7 3.357(28) . 1_555 N
O9 O7 5.654(24) . 2_645 N
O9 O7 5.868(23) . -2_566 N
O9 O8 3.937(31) . 1_555 N
O9 O8 4.128(31) . 1_655 N
O9 O8 2.958(19) . -1_656 N
O9 O9 3.06(4) . -1_656 N
O9 Ge1 4.255(21) . 1_555 N
O9 Ge1 4.182(19) . 2_645 N
O9 Ge1 5.715(24) . -1_656 N
O9 Ge1 5.692(21) . -2_666 N
O9 Ge2 4.123(24) . 1_555 N
O9 Ge2 3.991(23) . 2_645 N
O9 Ge2 4.204(20) . -2_566 N
O9 O10 4.92(5) . 1_545 N
O9 O10 4.99(5) . 1_645 N
O9 O10 5.77(5) . 2_545 N
O9 O10 5.73(5) . 2_645 N
O9 O10 4.16(5) . -1_666 N
Ge1 Ga1 5.266(31) . -1_555 N
Ge1 Ga1 5.999(7) . -2_565 N
Ge1 Ga1 5.999(7) . -2_566 N
Ge1 Ga2 3.875(23) . 1_455 N
Ge1 Ga2 4.189(23) . 1_555 N
Ge1 Ga2 5.571(11) . -1_655 N
Ge1 Ga2 5.936(27) . -2_465 N
Ge1 La1 3.933(25) . -1_656 N
Ge1 La1 3.842(22) . -2_565 N
Ge1 La2 3.718(19) . 1_554 N
Ge1 La2 3.681(21) . -1_556 N
Ge1 La2 3.615(20) . -2_565 N
Ge1 La3 3.372(20) . 1_555 N
Ge1 La3 3.792(20) . -2_565 N
Ge1 La4 5.080(19) . 1_455 N
Ge1 La4 4.888(22) . 2_655 N
Ge1 La4 3.480(21) . -2_465 N
Ge1 O1 4.272(24) . 1_454 N
Ge1 O1 4.780(25) . -1_656 N
Ge1 O1 3.907(22) . -2_465 N
Ge1 O1 4.920(22) . -2_565 N
Ge1 O2 4.535(21) . 1_554 N
Ge1 O2 5.913(23) . -1_556 N
Ge1 O2 1.856(22) . -2_565 N
Ge1 O3 1.802(21) . 1_555 N
Ge1 O3 5.840(20) . 2_555 N
Ge1 O3 4.607(20) . -1_555 N
Ge1 O4 1.811(23) . 1_554 N
Ge1 O4 5.123(26) . -1_556 N
Ge1 O4 4.280(22) . -2_565 N
Ge1 O5 5.802(33) . 1_455 N
Ge1 O5 2.303(33) . 1_555 N
Ge1 O5 5.572(28) . -2_566 N
Ge1 O6 4.161(31) . 1_454 N
Ge1 O6 4.573(27) . 1_554 N
Ge1 O6 5.314(31) . -1_656 N
Ge1 O6 4.563(31) . -2_565 N
Ge1 O7 4.122(29) . 1_455 N
Ge1 O7 4.668(28) . 1_555 N
Ge1 O7 4.559(22) . 2_655 N
Ge1 O7 4.545(23) . -1_655 N
Ge1 O8 4.064(25) . 1_555 N
Ge1 O8 3.959(25) . 2_555 N
Ge1 O8 4.246(23) . -2_565 N
Ge1 O9 4.255(21) . 1_555 N
Ge1 O9 4.182(19) . 2_655 N
Ge1 O9 5.715(24) . -1_656 N
Ge1 O9 5.692(21) . -2_465 N
Ge1 Ge1 5.266(31) . -1_555 N
Ge1 Ge1 5.999(7) . -2_565 N
Ge1 Ge1 5.999(7) . -2_566 N
Ge1 Ge2 3.875(23) . 1_455 N
Ge1 Ge2 4.189(23) . 1_555 N
Ge1 Ge2 5.571(11) . -1_655 N
Ge1 Ge2 5.936(27) . -2_465 N
Ge1 O10 5.973(35) . 1_545 N
Ge1 O10 1.94(5) . 2_545 N
Ge1 O10 5.64(4) . -1_565 N
Ge1 O10 5.539(33) . -2_565 N
Ge2 Ga1 4.189(23) . 1_555 N
Ge2 Ga1 3.875(23) . 1_655 N
Ge2 Ga1 5.571(11) . -1_655 N
Ge2 Ga1 5.936(27) . -2_666 N
Ge2 Ga2 5.433(30) . -1_655 N
Ge2 Ga2 5.982(6) . -2_565 N
Ge2 Ga2 5.982(6) . -2_566 N
Ge2 La1 3.775(20) . 1_554 N
Ge2 La1 3.835(23) . -1_656 N
Ge2 La1 3.609(21) . -2_565 N
Ge2 La2 3.818(21) . -1_656 N
Ge2 La2 3.797(19) . -2_665 N
Ge2 La3 4.880(20) . 2_655 N
Ge2 La3 3.510(19) . -2_565 N
Ge2 La4 3.402(20) . 1_555 N
Ge2 La4 3.650(21) . -2_565 N
Ge2 O1 4.683(27) . 1_554 N
Ge2 O1 1.801(25) . -2_565 N
Ge2 O2 4.525(21) . 1_554 N
Ge2 O2 4.682(22) . -1_656 N
Ge2 O2 4.487(22) . -2_565 N
Ge2 O2 4.367(23) . -2_665 N
Ge2 O3 4.374(26) . 1_555 N
Ge2 O3 4.478(25) . 1_655 N
Ge2 O3 4.411(19) . 2_655 N
Ge2 O3 4.769(21) . -1_655 N
Ge2 O3 5.992(21) . -2_565 N
Ge2 O4 4.432(25) . 1_554 N
Ge2 O4 4.398(26) . 1_654 N
Ge2 O4 5.339(29) . -1_656 N
Ge2 O4 4.324(24) . -2_665 N
Ge2 O5 1.943(34) . 1_555 N
Ge2 O5 5.374(26) . -1_655 N
Ge2 O5 5.579(26) . -2_565 N
Ge2 O6 1.669(26) . 1_554 N
Ge2 O6 5.224(31) . -1_656 N
Ge2 O6 4.418(26) . -2_565 N
Ge2 O7 1.788(24) . 1_555 N
Ge2 O7 4.491(28) . -1_655 N
Ge2 O8 4.308(26) . 1_655 N
Ge2 O8 3.982(25) . 2_655 N
Ge2 O8 5.646(26) . -1_656 N
Ge2 O8 5.711(27) . -2_565 N
Ge2 O8 5.941(27) . -2_665 N
Ge2 O9 4.123(24) . 1_555 N
Ge2 O9 3.991(23) . 2_655 N
Ge2 O9 4.204(20) . -2_565 N
Ge2 Ge1 4.189(23) . 1_555 N
Ge2 Ge1 3.875(23) . 1_655 N
Ge2 Ge1 5.571(11) . -1_655 N
Ge2 Ge1 5.936(27) . -2_666 N
Ge2 Ge2 5.433(30) . -1_655 N
Ge2 Ge2 5.982(6) . -2_565 N
Ge2 Ge2 5.982(6) . -2_566 N
Ge2 O10 2.14(5) . 2_645 N
Ge2 O10 5.42(4) . -1_666 N
O10 Ga1 5.973(35) . 1_565 N
O10 Ga1 1.94(5) . 2_555 N
O10 Ga1 5.64(4) . -1_565 N
O10 Ga1 5.539(33) . -2_566 N
O10 Ga2 2.14(5) . 2_655 N
O10 Ga2 5.42(4) . -1_666 N
O10 La1 4.36(4) . 2_656 N
O10 La1 4.91(5) . -1_566 N
O10 La1 4.79(5) . -1_666 N
O10 La2 4.39(4) . 2_556 N
O10 La2 2.774(32) . -1_566 N
O10 La2 3.842(35) . -2_565 N
O10 La3 4.74(4) . 1_565 N
O10 La3 4.22(5) . 2_555 N
O10 La3 4.85(5) . -1_566 N
O10 La3 4.65(5) . -1_666 N
O10 La4 4.69(4) . 1_465 N
O10 La4 4.17(4) . 2_655 N
O10 La4 2.51(4) . -1_666 N
O10 O1 3.91(4) . 2_656 N
O10 O1 2.32(4) . -1_666 N
O10 O1 5.70(4) . -2_465 N
O10 O2 5.55(5) . 2_556 N
O10 O2 5.70(5) . 2_656 N
O10 O2 2.53(5) . -1_566 N
O10 O2 5.60(4) . -2_565 N
O10 O3 4.410(35) . 1_565 N
O10 O3 3.17(5) . 2_555 N
O10 O3 4.594(33) . -2_566 N
O10 O4 2.55(4) . 2_556 N
O10 O4 3.866(34) . -1_566 N
O10 O4 5.45(4) . -2_565 N
O10 O4 5.85(4) . -2_575 N
O10 O5 4.11(6) . 2_555 N
O10 O5 3.98(6) . 2_655 N
O10 O5 5.97(6) . -1_565 N
O10 O5 5.74(6) . -1_666 N
O10 O6 2.50(6) . 2_656 N
O10 O6 5.69(6) . -1_566 N
O10 O6 5.65(5) . -1_666 N
O10 O7 4.54(4) . 1_465 N
O10 O7 3.07(4) . 2_655 N
O10 O7 5.56(4) . -1_666 N
O10 O7 5.91(4) . -2_466 N
O10 O7 5.95(5) . -2_566 N
O10 O8 2.835(34) . 1_565 N
O10 O8 4.18(4) . 2_555 N
O10 O8 4.24(5) . -1_566 N
O10 O9 4.99(5) . 1_465 N
O10 O9 4.92(5) . 1_565 N
O10 O9 5.77(5) . 2_555 N
O10 O9 5.73(5) . 2_655 N
O10 O9 4.16(5) . -1_666 N
O10 Ge1 5.973(35) . 1_565 N
O10 Ge1 1.94(5) . 2_555 N
O10 Ge1 5.64(4) . -1_565 N
O10 Ge1 5.539(33) . -2_566 N
O10 Ge2 2.14(5) . 2_655 N
O10 Ge2 5.42(4) . -1_666 N
O10 O10 5.8458(7) . -2_575 N
O10 O10 5.8458(7) . -2_576 N
